Surface Science 565 (2004) 151–162 www.elsevier.com/locate/susc
A.P. Grosvenor a,b,*, B.A. Kobe a, N.S. McIntyre a,b a Surface Science Western, Room G-1, Western Science Centre, The University of Western Ontario, London, Ont., Canada N6A 5B7 b Department of Chemistry, The University of Western Ontario, London, Ont., Canada N6A5B7
Received 22 March 2004; accepted for publication 21 June 2004 Available online 21 July 2004
TM Oxidation of iron (Fe) by oxygen (O2) at low pressures was investigated using XP spectra and QUASES Analyze and Generate software programs. The results indicated that the oxide ﬁlms produced after short oxygen exposure times contained a mixture of magnetite (Fe3O4) and maghemite (c-Fe2O3) without distinct interfaces between the two being seen. Further investigation suggested that a reaction mechanism involving cationic diﬀusion was mostly responsible for the formation of Fe3O4, while a mechanism involving anionic diﬀusion was responsible for c-Fe2O3 growth. The kinet- ics of the overall reaction were also investigated and found to follow a direct logarithmic relationship with increasing time. The rates of oxide growth were calculated for diﬀerent pressures studied at the same temperature and found to be the same. This observation was used to conclude that the rate-limiting step was the formation of a thin oxide ﬁlm by place-exchange and not anionic or cationic diﬀusion. 2004 Elsevier B.V. All rights reserved.
Keywords: X-ray photoelectron spectroscopy; Iron; Oxidation; Tunneling
1. Introduction the past [1–9]. Exposure of iron to low pressures of dry oxygen gas at room temperature results in The near surface structures produced during an oxide that has been reported to consist qualita- oxidation of iron have received great attention in tively of a layer of Fe3O4 covered by a second layer of c-Fe2O3 [4–6]. Other researchers examining the oxidation of single crystal Fe(100) have suggested * Corresponding author. Surface Science Western, Room G- that a mixture of oxides rather than distinct oxide 1, Western Science Centre, The University of Western Ontario, London, Ont., Canada N6A 5B7. Tel.: +1 519 661 2173/2111; layers are found . Kinetic studies performed by fax: +1 519 661 3709. Graham et al.  using a manometric method to E-mail address: [email protected] (A.P. Grosvenor). measure oxygen uptake at temperatures between
0039-6028/$ - see front matter 2004 Elsevier B.V. All rights reserved. doi:10.1016/j.susc.2004.06.210 152 A.P. Grosvenor et al. / Surface Science 565 (2004) 151–162
25 and 300 C found that the oxide formation fol- length and the energy loss function (inelastic elec- lowed a logarithmic function with increasing time. tron scattering cross-section) used. The initial oxi- The oxide in this study was assumed to be uniquely dation study of Fe using several pressures of O2 Fe3O4 and the amount of oxide formed was found  showed that the oxide layer did, in fact, con- to increase as the surfaces were changed from sin- tain a layered mixture of the oxides Fe3O4 and c- gle crystal to polycrystalline . These kinetic re- Fe2O3. sults have been conﬁrmed at temperatures below This paper reports a comprehensive study of the 200 C using XPS . Above 200 C, however, eﬀect of time, temperature and pressure on the plots of oxide thickness versus oxygen exposure growth of surface oxides during exposure of poly- have shown a greatly increased slope indicating a crystalline Fe to O2. The initiation of metal oxida- probable change in mechanism . Oxidation tion at low temperature has been suggested to studies of Fe carried out in O2 at pressures of less result from ﬁeld induced electron transport/tunnel- than 1 · 105 Pa and temperatures ranging from ling under constant potential from the metal 800 to 1000 C have indicated that the oxidation through an existing thin oxide ﬁlm to adsorbed kinetics obeyed a parabolic law . oxygen . The oxide initially grows quickly, with X-ray photoelectron spectroscopy (XPS) has the rate ﬂattening out when the potential across been used heavily to determine surface oxide com- the layer starts to become signiﬁcantly low . position and to measure changes in oxide thickness From this model, an inverse logarithmic growth [10,12–14]. In the past, XPS has had limited capac- versus time relationship has been derived: ity to probe compositions and structures beneath W qaE dx ð Þ the outermost oxide and to provide a well deﬁned ¼ NXme kT ð1Þ measure of the interfaces that are known or ex- dt pected to be present following a reaction of metal where x = oxide thickness, t = time, N = potential and oxygen. However, the development of meth- number of mobile ions, X = oxide volume per mo- ods to analyze the extrinsic loss structure present bile ion, m = atomic vibration frequency, W = en- in all XP spectra [15,16] appears poised to increase ergy barrier to ion movement into the oxide, the density of information available on surface q = ionic charge (Ze), a = half the ion jump dis- structures. Speciﬁcally, such methods seem capa- tance, E = the electric ﬁeld (V/x), k = BoltzmannÕs ble of providing much improved deﬁnition, both constant, and T = the temperature at which the to the identiﬁcation of oxide structures as well as reaction occurs . The integrated equation is usu- their thicknesses. ally represented as 1 ¼ kT ln t + constant . Research in this laboratory using XPS and x qaV QUASESTM Generate and Analyze  software Direct logarithmic kinetics proposed by Eley programs has shown that the QUASESTM algo- and Wilkinson  also allows for an electron tun- rithms are suitable for studying the oxidation of nelling mechanism, but for ﬁlm growth under con- Fe . These algorithms are used to model the stant ﬁeld conditions: extrinsic loss structures found in XP spectra, and dx 0:6 bx E 0:6 cx ¼ aP e ¼ Ae RT P e RT ð2Þ from this, determine the depth at which the loss sig- dt nals originate . ‘‘Analyze’’ models the extrinsic background of a photoelectron peak, allowing one where A = the pre-exponential value, E = activa- to determine the range of depth at which the bulk tion energy, P = reaction pressure, T = tempera- structure originated. ‘‘Generate’’, on the other ture, x = thickness of the oxide at time t, and hand, allows the experimental spectra to be mod- c = increase in activation free energy with thick- elled using various combinations of reference spec- ness of the oxide ﬁlm . The inclusion of P in tra whose extrinsic backgrounds have been altered the equation indicates the importance of the oxy- based on the depth at which they are found within gen concentration to the reaction and is thus more the surface [17,18]. The accuracy of the thickness appropriate for a mechanism involving anion dif- determined is dependent upon the attenuation fusion . A.P. Grosvenor et al. / Surface Science 565 (2004) 151–162 153
This paper describes the oxidation of Fe under . The vacuum in the reaction chamber was con- low temperature ( 6 150 C) and pressure condi- trolled using multiple turbo-molecular pumps. tions. Speciﬁc attention will be paid to the individ- ual reactions governing the growth of Fe3O4 and 2.2. Reactions c-Fe2O3. The kinetics of the reaction will be shown to be modelled best using a logarithmic equation. To oxidize the clean Fe surface, medical grade oxygen (Praxair) dried by passage through a silica gel column (6–8 mesh, EM Science) was used. The 2. Experimental polyvinyl tube used to carry the oxygen into the instrument from the gas cylinder was pumped 2.1. Sample preparation out under vacuum for 24 h prior to beginning the study to remove as much adsorbate contami- Pure polycrystalline iron rod (99.995%) from nation as possible. After introduction into the vac- Alfa-Aesar was cut into 3.4 mm disks using a dia- uum chamber where dosing was performed, the mond saw with one surface being polished to a samples were exposed to the reactant gas for 120 2 2 mirror ﬁnish using 0.05 lm c-Al2O3. Samples were s at pressures of 1.3 · 10 , 1.3, and 1.3 · 10 Pa degreased in methanol using an ultrasonic cleaner measured using a Pirani gauge and temperatures and then loaded into a Kratos AXIS Ultra XPS of 27 ± 2 and 150 ± 1 C. The total dose in Lang- for oxygen treatment and analysis. All samples muirs (L) was calculated by using the average pres- were cleaned again in the vacuum chamber of the sure of O2 that the surface experienced. The Kratos spectrometer ﬁrst by sputter cleaning the reaction kinetics were also observed at oxygen dos- surface for 10 min using a 4 kV Ar+ ion beam, then ing pressures of 1.3 · 10 2 and 1.3 Pa. The expo- by annealing in vacuum at 600 C for 30 min. sure times were 20, 200, and 2000 s with the After in vacuo cleaning, all samples were analyzed temperature held at 27 ± 1 C. When oxidizing by XPS to conﬁrm that all contaminate species (C, the samples, a certain amount of time was always Na, etc.) had been removed and that no oxides required to increase the O2 pressure to the wanted remained. value. Although the amount of O2 to which the After the surface was determined to be free of surface was exposed was very small, it cannot be oxides, it was transferred into another vacuum ruled out that some oxide did in fact form during chamber of the XPS where the dosing experiments this time period. After dosing, the samples were re- were performed. Before the sample was placed in turned to the analytical chamber and analyzed this chamber, a residual gas analyzer was ﬁrst used using the following conditions; monochromatic to determine the gas partial pressures in the cham- Al Ka X-ray source, binding energy (BE) ber. Although water vapour had the highest partial range = 1100–0 eV, step size = 0.7 eV, pass pressure (typically 10 6 Pa) of the residual gases, E = 160 eV, sweep time = 180 s, and number of 4 this was 10 times lower than the O2 pressures used sweeps = 8. High resolution spectra were also ta- during reaction (>10 2 Pa). To rule out that any of ken for Fe 2p, O 1s, and C 1s using a 20–40 eV the reaction products found during this study were window, depending on the peak analyzed, and a from the reaction of Fe and water vapour, a clean pass energy of 40 eV. The transfer lens was used Fe disk was exposed to the residual gases found in in electrostatic mode due to the ferromagnetic the reaction chamber for 2 min and than analyzed properties of Fe. by XPS. No oxide or hydroxide species were found indicating that the background contamination pre- 2.3. Data analysis sent in the reaction chamber was not concentrated enough to react with the Fe. This result follows All spectra were ﬁrst analyzed using the Casa- those shown in a previous study which indicated XPS software . After being oxidized, all of that water vapour is much less reactive towards the surfaces analyzed were found to contain small Fe than oxygen gas is after equivalent exposures concentrations of adventitious C on the surface. 154 A.P. Grosvenor et al. / Surface Science 565 (2004) 151–162
Peak shifts due to any apparent charging were nor- tal spectra located between kinetic energies of 720 malized with the C 1s peak set to 284.8 eV. The Fe and 750 eV. Further information on the methodol- 2p high resolution spectra were ﬁtted using Gup- ogy used when ﬁtting the spectra using either Gen- ta–Sen multiplet peaks [22–25]. The Fe3+/Fe2+ erate or Analyze can be found in Ref. . peak ratio was allowed to vary since Fe2O3 is The IMFP values used for the Fe 2p photoelec- known to form, as well as Fe3O4, in these condi- trons from the metal and oxides were: kFe = 1.57 tions [3,18]. Any Fe metal component found nm, kFe3O4 = 1.65 nm, and kFe2O3 = 1.65 nm. Dur- (BE = 707 eV) was ﬁtted using a Doniach and Sun- ing our initial investigations , an experimental jic asymmetric synthetic peak corresponding to attenuation length was determined for the Fe 2p interactions of conduction electrons with the core photoelectron of the c-Fe2O3/Fe3O4 oxide. This hole . The peak full width at half maximum was done by an independent measurement of this (FWHM) was generally held to be between 1.0 oxide thickness using nuclear reaction analysis and 1.2 eV. The width used was determined by (NRA). The value of the attenuation length deter- matching the low BE slope of the synthetic peak mined from the NRA experiment (1.38 nm) was to that of the spectrum. The O 1s high resolution found to be approximately 20% lower than the spectra were also examined for the presence of IMFP value calculated using the TPP-2M equa- O2 near 530 eV [4,27] and other oxygen species tion (1.65 nm) . All thicknesses listed below at binding energies extending from 531 to 532 eV. were altered to reﬂect this diﬀerence.
2.4. QUASESTM 3. Results To determine the approximate oxide layer TM depth, QUASES Analyze was used to assess 3.1. Eﬀects of O2 dose over a range of pressures: 27 the oxide thickness from the O 1s extrinsic loss and 150 C structure. The attenuation lengths used in the TM QUASES computations were approximated by Fig. 1 shows the Fe 2p3/2 photoelectron spec- inelastic mean free path (IMFP, k) values deter- trum following oxidation at pressures of 0, 2 2 mined using the TPP-2M equation . The value 1.3 · 10 , 1.3, and 1.3 · 10 Pa O2 at 27 C. The for O 1s was determined using Fe3O4 as the model oxide portion of the spectra was consistently ob- compound and a kinetic energy of 956 eV. The served to contain the oxide species Fe3O4 and IMFP (kO1 s) determined was 1.93 nm. The univer- Fe2O3, with no detectable presence of FeO. Fig. sal cross-section developed by Tougaard  was 2 shows the equivalent Fe 2p3/2 spectra for these used for all species analyzed. pressures at an oxidation temperature of 150 C; Generate was used to determine the depth of the eﬀect of the higher temperature is clearly individual oxide layers using the Fe 2p region on evident. the basis of the appropriate reference spectra ob- For all oxygen exposures, the extrinsic back- tained previously. Reference samples used were ground associated with the O 1s line was ﬁrst ana- the same as those discussed in Ref. . Spectra lyzed to determine the distribution of the oxygen from the reference compounds were all used either density as a function of depth. This was done using separately or in combination to model the experi- the QUASESTM Analyze software program and a mental spectra under consideration. The surfaces k value of 1.93 nm for the O 1s electrons. Fig. 3 were always modelled in such a way that the shows a typical analysis of the extrinsic back- Fe(0) metal spectra remained as the bulk, overlaid ground including the separation of the intrinsic by Fe2+ compounds, followed by the Fe3+ com- portion of the spectrum. pounds that were closest to the surface. A spec- From this O 1s study, a total thickness of oxy- trum was deemed to have been adequately ﬁtted gen through the surface structure was determined. if the model spectra almost or completely overlaid This would include oxygen formed as a solid oxide the extrinsic background region of the experimen- as well as interstitial oxygen within the metal and A.P. Grosvenor et al. / Surface Science 565 (2004) 151–162 155